Giant phonon-induced conductance in
scanning tunnelling spectroscopy of
YUANBO ZHANG 1 *, VICTOR W. BRAR 1,2 , FENG WANG 1 , CAGLAR GIRIT 1,2 , YOSSI YAYON 1 ,
MELISSA PANLASIGUI 1 , ALEX ZETTL 1,2 AND MICHAEL F. CROMMIE 1,2 *
1 Department of Physics, University of California at Berkeley, Berkeley, California 94720, USA
2 Materials Sciences Division, Lawrence Berkeley Laboratory, Berkeley, California 94720, USA
*e-mail: firstname.lastname@example.org; email@example.com
Published online: 20 July 2008; doi:10.1038/nphys1022
The honeycomb lattice of graphene is a unique two-dimensional
system where the quantum mechanics of electrons is equivalent
to that of relativistic Dirac fermions 1,2 . Novel nanometre-scale
behaviour in this material, including electronic scattering 3,4 ,
spin-based phenomena 5 and collective excitations 6 , is predicted
to be sensitive to charge-carrier density. To probe local,
carrier-density-dependent properties in graphene, we have
carried out atomically resolved scanning tunnelling spectroscopy
measurements on mechanically cleaved graphene flake devices
equipped with tunable back-gate electrodes. We observe an
unexpected gap-like feature in the graphene tunnelling spectrum
that remains pinned to the Fermi level (E F ) regardless of
graphene electron density. This gap is found to arise from a
suppression of electronic tunnelling to graphene states near E F
and a simultaneous giant enhancement of electronic tunnelling
at higher energies due to a phonon-mediated inelastic channel.
Phonons thus act as a ‘floodgate’ that controls the flow of
tunnelling electrons in graphene. This work reveals important
new tunnelling processes in gate-tunable graphitic layers.
Graphene provides an ideal platform for the local study of
high-mobility two-dimensional (2D) electrons because it can be
fabricated on top of an insulating substrate. The availability
of a back-gate electrode makes graphene the first gate-tunable
2D system directly accessible to scanning probe measurement
(Fig. 1a). Previous experiments have demonstrated the power
of scanning tunnelling microscopy (STM) to probe the local
electronic structure of graphene grown epitaxially on SiC (refs 7–9).
That system, however, cannot be easily gated, and questions remain
as to the influence of the SiC substrate on the graphene layer 6,10 .
Mechanically cleaved graphene is a desirable alternative to graphene
grown on SiC because it can be readily gated and placed on wellcontrolled
substrates (Fig. 1a), thus making it useful for extracting
intrinsic graphene properties.
The STM topography of a gated graphene flake device is
shown in Fig. 2a. Corrugations with a lateral dimension of a few
nanometres and a vertical dimension of ∼1.5 Å (r.m.s. value over
a 60×60 nm 2 area) are observed, probably due to roughness in the
underlying SiO 2 (refs 11,12). The graphene honeycomb lattice can
be clearly resolved on top of the surface corrugation, as seen more
clearly in Fig. 2b.
Raman intensity (a.u.)
Wavenumber (cm –1 )
Figure 1 Local probe geometry of gated graphene flake device. a, Optical image
of a mechanically cleaved gated graphene flake (dark triangle in centre) accessed by
STM tip (tip is sketched). The graphene is contacted by gold electrodes and a
back-gate voltage (V g ) is applied to the underlying Si substrate. b, Raman spectrum
of the graphene sample in a showing a single peak at wavenumber ∼2,700 cm −1 , a
clear signature for monolayer graphene.
We explored the local electronic structure of these graphene
flake devices using dI/dV measurements at zero gate voltage,
as shown in Fig. 2c. Strikingly, the spectrum shows a ∼130 mV
gap-like feature centred at the Fermi energy, E F , as opposed to
the linear density of states that might be expected from elastic
tunnelling to a Dirac cone. A local minimum in the tunnelling
conductance spectrum can also be seen at V D = −138 mV, making
the spectrum asymmetric about E F . Close examination of the
low-bias spectrum (Fig. 2c, inset) reveals that the tunnelling
conductance does not go to absolute zero in the gap region.
These observations were reproduced on more than eight different
flake devices, and the gap feature was observed in every spectrum
acquired with calibrated STM tips (more than 30 different tips).
The gap feature was seen to be independent of location on a
sample, although the energy position of the adjacent dip feature,
V D , varied with tip location. This observation (together with the
fact that a similar gap feature of the same size was seen on
a graphene/SiC sample 9 ) is evidence against substrate-induced
effects as the origin of the gap feature, because such effects would
nature physics VOL 4 AUGUST 2008 www.nature.com/naturephysics 627
© 2008 Macmillan Publishers Limited. All rights reserved.
V g = +60 V
–1.8 Å 2.1 Å
–0.1 Å 0.1 Å
–0.1 0 0.1
Sample bias (V)
–0.4 –0.2 0 0.2 0.4
Sample bias (V)
Figure 2 Graphene surface topography and differential conductance (dI/dV )
spectrum. a, Constant-current STM topograph (1 V, 50 pA) of a graphene flake
above a SiO 2 substrate. b, Close-up constant-current STM topograph (0.15 V, 40 pA)
of the graphene honeycomb lattice. c, dI/dV spectrum of graphene at zero gate
voltage. The spectrum was acquired at a nominal junction impedance of 5 G
(0.5 V, 100 pA). The gap width and the adjacent conductance minimum location
(at V D ) were not sensitive to STM tip height over an impedance range of 1–100 G.
Inset: A high-resolution dI/dV spectrum emphasizing the central gap-like feature.
–0.4 –0.2 0 0.2 0.4 0.6
Sample bias (V)
imply a gap that depends on spatial location as well as the type
Changing the device gate voltage, V g , causes the graphene Dirac
point (E D ) to shift energetically relative to E F , inducing a 2D
charge-carrier density of n = αV g , where α = 7.1 × 10 10 cm −2 V −1
(estimated using a simple capacitor model 1,2 ). STM dI/dV spectra
taken at the same location on graphene with gate voltages ranging
from V g = −60 to +60 V are shown in Fig. 3a. The width and
energy position of the central gap feature do not show any
dependence on gate voltage, but the conductance minimum at V D
shifts monotonically with gate voltage, and even switches polarity
(red arrows, Fig. 3a).
To further characterize the mysterious central gap feature,
we measured both the temperature dependence and the effective
barrier for electrons tunnelling into graphene. As shown in Fig. 4a,
no significant temperature dependence is observed in graphene
dI/dV spectra measured at T = 4.8 and 77.5 K (this lack of
temperature dependence was observed for −60 V < V g < +60 V).
Tunnel barrier measurements were carried out by measuring
the STM tunnel current as a function of tip–sample separation
(z) at constant bias for voltages inside and outside the gap,
and identical measurements were also carried out on a gold
sample using the same tip as a calibration. STM tunnel current
depends exponentially on z, I ∝ e −z/l , and the decay length (l)
gives a measure of the effective tunnel barrier. l was obtained
by fitting I versus z measurements at large z (tunnel junction
resistance > 30 G) with an exponential function. As seen in
Fig. 4b, l for graphene is comparable to that observed in the
gold calibration data (l ≈ 0.45 Å) for biases outside the gap, but
E D (eV)
–60 –30 0 30 60
V g (V)
Figure 3 Gate-voltage dependence of graphene tunnelling spectra. a, dI/dV
spectra taken at the same point on the graphene surface for different gate voltages,
V g . Spectra are acquired at the same nominal junction impedance, 5 G (0.5 V,
100 pA). Curves are vertically displaced for clarity. Red arrows indicate the
gate-dependent positions of the adjacent conductance minimum, V D , outside the
gap feature. b, Energy position of the Dirac point, E D , as a function of applied gate
voltage (extracted from the conductance minimum in a using equation (1):
E D = e|V D |− ¯hω 0 ). E D and its associated uncertainty (which is smaller than the size
of the symbols) are obtained by fitting the minimum with polynomials. The black
curve is a fit to the data using the square-root dependence of E D on gate voltage.
The inset schematic diagrams show linear graphene energy bands when a gate
voltage is applied (filled states are orange).
decreases markedly to a value only half as large (l ≈ 0.25 Å) for
biases within the gap.
How do we interpret the anomalous graphene energy gap
behaviour and gate-voltage-dependent conductance minima?
A consistent picture emerges if we consider phonon-mediated
628 nature physics VOL 4 AUGUST 2008 www.nature.com/naturephysics
© 2008 Macmillan Publishers Limited. All rights reserved.
T = 4.8 K
T = 77.5 K
–0.2 0 0.2
Sample bias (V)
Decay length (Å)
–0.2 –0.1 0 0.1 0.2
Sample bias (V)
e – hω 0
Figure 4 Characterization of the Fermi level gap feature and inelastic electron
tunnelling mechanism. a, Graphene dI/dV conductance spectra measured at
T = 4.8 K and 77.5 K (no significant temperature dependence is observed).
b, Tunnel current decay length of graphene and Au(111) surfaces probed at different
bias voltages with the same STM tip. Error bars represent standard deviations of the
measurements. c, Inelastic electron tunnelling due to excitation with energy ¯hω 0 .
d, Wave-vector-dependent inelastic tunnelling mechanism involving graphene
phonon modes near the K point in reciprocal space.
inelastic tunnelling of electrons into the graphene flake
accompanied by a strong suppression of elastic tunnelling at E F .
In what follows, we first establish a general inelastic origin of
the central gap feature and we then discuss how our data can be
explained by a novel phonon-based inelastic excitation mechanism.
STM tunnel current is generally enhanced if the bias voltage is
high enough to provide tunnelling electrons with enough energy to
induce excitations that have some threshold energy ¯hω 0 (Fig. 4c) 13 .
This opens up a new inelastic tunnelling channel at bias voltages
of ±¯hω 0 /e, causing steps in dI/dV spectra that are symmetric
around E F and that lead to a gap-like feature with width 2¯hω 0 .
In the case of our graphene measurements, ¯hω 0 = 63 ± 2 meV
(this corresponds to one half of the voltage separation between
peak centres in d 2 I/dV 2 ). Strong evidence for such an inelastic
tunnelling mechanism in graphene (as opposed to some other gapinducing
mechanism) can be seen in our data by analysing the gatevoltage
dependence of the conductance minimum observed at V D .
If we assume that this minimum arises from inelastic tunnelling
to the graphene Dirac point (a minimum in the density of states),
then its energy location in our data (eV D ) should be offset by ¯hω 0
from its true energy location, E D , in the graphene band structure
(because each inelastically tunnelling electron loses energy ¯hω 0 ):
E D = e|V D |− ¯hω 0 . (1)
Because V D depends on gate voltage, this inelastic relation
enables us to directly plot E D versus V g , as shown in Fig. 3b.
Identification of the conductance minimum at V D with the Dirac
point energy, E D , can be confirmed √ by fitting this plot with the
expected dependence E D = ¯hv F πα|Vg − V 0 | as prescribed by the
graphene linear band structure 1,2 . Here, v F is the Fermi velocity of
graphene and V 0 is the shift of the Dirac point (in terms of gate
voltage) due to substrate doping. An excellent fit is obtained with
v F = 1.10±0.01×10 6 m s −1 and V 0 = −4.1±0.2 V, values that are
consistent with those of previous studies 1,2,14 . This unambiguously
identifies the observed conductance minimum at V D as the Dirac
point and simultaneously verifies a graphene inelastic tunnelling
channel as the origin of the central gap feature.
The question next arises as to what specific type of graphene
inelastic excitation we are observing that has energy ¯hω 0 ≈ 63 meV.
One possible attribution is the 67 meV out-of-plane acoustic
graphene phonon modes located near the K/K ′ points in reciprocal
space 15 . Electrons with energy less than this phonon threshold
energy tunnel elastically into graphene at E F (near the K point) with
only a low probability due to suppression of electronic tunnelling
into states with a large wave vector 16,17 . Once the threshold bias
voltage ±¯hω 0 /e is reached, however, tunnelling into K point
states is markedly enhanced (seen as more than a factor of 10
increase in tunnelling conductance) by the opening of a new
inelastic channel. In this new mechanism, an electron first tunnels
into the graphene σ ∗ band near the Ɣ point in reciprocal space
(a virtual transition as shown in Fig. 4d) before falling into an
available K point state on the π band through the emission of
a K ′ point out-of-plane phonon (to conserve crystal momentum
and energy). This phonon-mediated inelastic tunnelling process,
which involves momentum-conserving virtual transitions between
2D electronic bands, is distinctly different from previously studied
inelastic tunnelling in single molecules 13,18 or localized spins 19
where momentum is not a well-defined quantity owing to a lack
of translational symmetry (phonon-induced inelastic tunnelling
in single molecules typically leads to conductivity changes of the
order of only 1% in contrast to the factor of 10 seen here 18 ).
This is also different from band-structure-dependent tunnelling
in silicon 20 because the wave-vector dependence seen here is a
result of inelastic excitations that couple the unique electronic
band structure and phonon spectrum of graphene. A recent
calculation 21 by Wehling et al. confirms this general interpretation
through density functional theory. They find significant mixing
of the graphene σ and π electron bands due to the out-ofplane
phonon mode at K/K ′ , resulting in a strongly enhanced
inelastic electron tunnel current. We note that there are three
in-plane phonon modes at K/K ′ , but their contributions to this
process are insignificant owing to the symmetries of the σ and
π bands 22 .
This mechanism is strongly supported by our observed
wavefunction spatial decay rates. Within the observed energy gap
(at energies below the inelastic threshold), electrons have to tunnel
directly into graphene states with large crystal momentum parallel
to the surface (k ‖ = K or K ′ ). Such states tend to decay rapidly in
the vacuum region above a surface, because their evanescent local
density of states is expected to fall off as 16
LDOS(z,k ‖ ) ∝ e −z/l , l −1 = 2 2mφ/¯h 2 + k‖, 2 (2)
where φ is the workfunction and m is the mass of an electron.
This accounts for the strong suppression of tunnelling conductance
within the energy gap region and leads to the small decay length
observed in the low-bias elastic tunnelling channel. At voltages
outside the gap (at energies above the inelastic threshold), however,
electrons tunnel via virtual excitations to the σ ∗ -band states near
the Ɣ point which have k ‖ ≈ 0. Such states tend to extend further
into the vacuum, leading to a larger decay length. Using the
two measured decay lengths (∼0.45 Å for k ‖ = 0 and ∼0.25 Å
for k ‖ = K) combined with equation (2), we are able to extract
a workfunction of φ = 4.6 ± 0.2 eV and a graphene K point
wave vector K = 1.7 ± 0.4 Å −1 . These values agree well with
the known workfunction of graphite and the known graphene
nature physics VOL 4 AUGUST 2008 www.nature.com/naturephysics 629
© 2008 Macmillan Publishers Limited. All rights reserved.
K point wavevector K = 1.7 Å −1 . This behaviour explains why
the gap feature seen here is not observed by other experimental
techniques (such as angle-resolved photoemission spectroscopy
and transport measurements) that are not sensitive to the spatial
decay of the electron wavefunction at a surface. The observed
lack of temperature dependence in our dI/dV spectra can also
be explained by the fact that the K/K ′ phonon energy is so much
higher than k B T (k B is the Boltzmann constant).
It is possible to gain insight into the electron–phonon coupling
strength that underlies the inelastic tunnelling process observed
here. The ratio of phonon-mediated tunnelling conductance
at energies just outside the gap compared with elastic tunnel
conductance at energies inside the gap can be approximated as
follows (see the Supplementary Information):
( ) /( )
k ‖ =0 −l−1 k ‖ =K
Here, V e–ph is the intrinsic graphene electron–phonon coupling
matrix element connecting electronic states at the Ɣ and K
points in reciprocal space and E σ is the energy of intermediate
states near the Ɣ point on the σ ∗ band (E σ ∼ 4 eV; ref. 23).
If we take the STM tip height as z ≈ 5 Å (estimated from
the tip–sample junction impedance ≈ 2 G) and use our
measured ratio of (dI/dV ) out /(dI/dV ) in ≈ 13, then equation (3)
enables us to extract an experimental electron–phonon coupling
strength V el–ph ≈ 0.4 eV, consistent with a theoretical estimate
of V el–ph ≈ 0.5 eV based on a simple tight-binding model 22 (see
equations 5.16, 5.18 and 5.20 and figure 5–9 in ref. 24). Our
experimental value of V el–ph , however, should only be taken as a very
rough estimate because the absolute tip-height above graphene, z,
is not directly measured.
In summary, we have demonstrated the ability to measure
atomically resolved local electronic structure of a graphene flake
device while changing its charge-carrier density using a back gate.
The resulting graphene spectra exhibit a prominent gap-like feature
that arises from a unique phonon-mediated inelastic tunnelling
process that is intrinsic to graphene. Phonons thus serve as a
‘floodgate’ in graphene by promoting electronic tunnelling above a
phonon threshold energy. The resulting nonlinear tunnelling I–V
behaviour will impact future graphene device applications that use
electron tunnelling processes.
Our graphene monolayers were prepared in a similar fashion as in ref. 25.
Monolayers of graphene were identified using an optical microscope, and
were subsequently confirmed using Raman spectroscopy (Fig. 1b) 26,27 . Gold
electrodes (30 nm) were attached to graphene using direct deposition through
a stencil mask for surface cleanliness. The gold contacts remained Ohmic up
to a source–drain voltage of 500 mV (contact resistance < 300 ). Heavily
doped Si under the SiO 2 layer was used as a back gate, enabling us to vary the
carrier density in the graphene (Fig. 1a). All graphene samples were annealed
at 400 ◦ C in ultrahigh vacuum for ∼10 h to ensure surface cleanliness before
Our STM measurements were carried out in an Omicron low-temperature
STM at T = 4.8 K and in an ultrahigh-vacuum environment with
base pressure < 10 −11 mbar. STM measurements were conducted with
chemically etched metal STM tips made of tungsten or platinum/iridium alloy.
To ensure that our STM tips were free of anomalies in their electronic structure,
we calibrated the tips by carrying out tunnelling differential conductance
(dI/dV) measurements on a clean Au(111) surface both before and after
graphene measurement. This calibration is crucial for obtaining reproducible
intrinsic tunnelling spectra on graphene because tip contamination is known
to induce spurious artefacts 28 (see the Supplementary Information). dI/dV
spectra were measured through lock-in detection 9 .
Received 6 February 2008; accepted 5 June 2008; published 20 July 2008.
1. Novoselov, K. S. et al. Two-dimensional gas of massless Dirac fermions in graphene. Nature 438,
2. Zhang, Y., Tan, Y.-W., Stormer, H. L. & Kim, P. Experimental observation of the quantum Hall effect
and Berry’s phase in graphene. Nature 438, 201–204 (2005).
3. Katsnelson, M. I., Novoselov, K. S. & Geim, A. K. Chiral tunnelling and the Klein paradox in
graphene. Nature Phys. 2, 620–625 (2006).
4. Cheianov, V. V., Fal’ko, V. & Altshuler, B. L. The focusing of electron flow and a Veselago lens in
graphene p–n junctions. Science 315, 1252–1255 (2007).
5. Son, Y. W., Cohen, M. L. & Louie, S. G. Half-metallic graphene nanoribbons. Nature 444,
6. Bostwick, A., Ohta, T., Seyller, T., Horn, K. & Rotenberg, E. Quasiparticle dynamics in graphene.
Nature Phys. 3, 36–40 (2007).
7. Rutter, G. M. et al. Scattering and interference in epitaxial graphene. Science 317, 219–222 (2007).
8. Mallet, P. et al. Electron states of mono- and bilayer graphene on SiC probed by scanning-tunneling
microscopy. Phys. Rev. B 76, 041403 (2007).
9. Brar, V. W. et al. Scanning tunneling spectroscopy of inhomogeneous electronic structure in
monolayer and bilayer graphene on SiC. Appl. Phys. Lett. 91, 122102 (2007).
10. Zhou, S. Y. et al. Substrate-induced bandgap opening in epitaxial graphene. Nature Mater. 6,
11. Ishigami, M., Chen, J. H., Cullen, W. G., Fuhrer, M. S. & Williams, E. D. Atomic structure of graphene
on SiO 2. Nano Lett. 7, 1643–1648 (2007).
12. Stolyarova, E. et al. High-resolution scanning tunneling microscopy imaging of mesoscopic graphene
sheets on an insulating surface. Proc. Natl Acad. Sci. 104, 9209–9212 (2007).
13. Lambe, J. & Jaklevic, R. C. Molecular vibration spectra by inelastic electron tunneling. Phys. Rev. 165,
14. Martin, J. et al. Observation of electron–hole puddles in graphene using a scanning single electron
transistor. Nature Phys. 4, 144–148 (2008).
15. Mohr, M. et al. Phonon dispersion of graphite by inelastic x-ray scattering. Phys. Rev. B 76,
16. Tersoff, J. & Hamann, D. R. Theory and application for the scanning tunneling microscope. Phys. Rev.
Lett. 50, 1998–2001 (1983).
17. Vitali, L. et al. Phonon and plasmon excitation in inelastic electron tunneling spectroscopy of
graphite. Phys. Rev. B 69, 121414(R) (2004).
18. Stipe, B. C., Rezaei, M. A. & Ho, W. Single-molecule vibrational spectroscopy and microscopy.
Science 280, 1732–1735 (1998).
19. Hirjibehedin, C. F., Lutz, C. P. & Heinrich, A. J. Spin coupling in engineered atomic structures.
Science 312, 1021–1024 (2006).
20. Stroscio, J. A., Feenstra, R. M. & Fein, A. P. Electronic-structure of the Si(111)2×1 surface by
scanning-tunneling microscopy. Phys. Rev. Lett. 57, 2579–2582 (1986).
21. Wehling, T. O., Grigorenko, I., Lichtenstein, A. I. & Balatsky, A. V. Phonon mediated tunneling into
graphene. Preprint at (2008).
22. Jiang, J. et al. Electron–phonon matrix elements in single-wall carbon nanotubes. Phys. Rev. B 72,
23. Sugawara, K., Sato, T., Souma, S., Takahashi, T. & Suematsu, H. Fermi surface and edge-localized
states in graphite studied by high-resolution angle-resolved photoemission spectroscopy. Phys. Rev. B
73, 045124 (2006).
24. Samsonidze, G. PhD thesis (Massachusetts Institute of Technology, Massachusetts, 2006).
25. Novoselov, K. S. et al. Two-dimensional atomic crystals. Proc. Natl Acad. Sci. 102,
26. Ferrari, A. C. et al. Raman spectrum of graphene and graphene layers. Phys. Rev. Lett. 97,
27. Gupta, A., Chen, G., Joshi, P., Tadigadapa, S. & Eklund, P. C. Raman scattering from high-frequency
phonons in supported n-graphene layer films. Nano Lett. 6, 2667–2673 (2006).
28. Tiedje, T., Varon, J., Deckman, H. & Stokes, J. Tip contamination effects in ambient pressure scanning
tunneling microscopy imaging of graphite. J. Vac. Sci. Technol. A 6, 372–375 (1988).
Supplementary Information accompanies this paper on www.nature.com/naturephysics.
We thank D.-H. Lee, S. Louie, A. Balatsky, J. Moore, C. H. Park, G. Samsonidze, D. Wegner,
L. Berbil-Bautista and C. Hirjibehedin for helpful discussions. This work was supported by the DOE
under contract No. DE-AC03-76SF0098. Y.Z. and F.W. acknowledge postdoctoral fellowships and
A.Z. acknowledges a professor fellowship, from the Miller Institute, UC Berkeley.
Reprints and permission information is available online at http://npg.nature.com/reprintsandpermissions.
Correspondence and requests for materials should be addressed to Y.Z. or M.F.C.
630 nature physics VOL 4 AUGUST 2008 www.nature.com/naturephysics
© 2008 Macmillan Publishers Limited. All rights reserved.